İSTANBUL TECHNICAL UNIVERSITY INSTITUTE OF SCIENCE AND TECHNOLOGY
IONIC CROSSLINKING OF COTTON FABRICS TO IMPROVE WRINKLE RECOVERY
Ph.D. Thesis by Umut Kıvanç ŞAHİN
Department : Textile Engineering Programme: Textile Engineering
İSTANBUL TECHNICAL UNIVERSITY INSTITUTE OF SCIENCE AND TECHNOLOGY
Ph.D. Thesis by Umut Kıvanç ŞAHİN
Date of submission : 28 January 2009 Date of defence examination: 24 April 2009
Supervisor (Chairman) : Assoc. Prof. Dr. Nevin Çiğdem GÜRSOY (ITU) Members of the Examining Committee : Prof. Dr. Peter HAUSER (NCSU)
Prof. Dr. Oya ATICI (ITU) Prof. Dr. Cevza CANDAN (ITU) Assoc. Prof. Dr. Mehmet KANIK (UU)
IONIC CROSSLINKING OF COTTON FABRICS TO IMPROVE WRINKLE RECOVERY
İSTANBUL TEKNİK ÜNİVERSİTESİ FEN BİLİMLERİ ENSTİTÜSÜ
DOKTORA TEZİ Umut Kıvanç ŞAHİN
Tezin Enstitüye Verildiği Tarih : 28 Ocak 2009 Tezin Savunulduğu Tarih : 24 Nisan 2009
Tez Danışmanı : Doç. Dr. Nevin Çiğdem GÜRSOY (İTÜ) Diğer Jüri Üyeleri : Prof. Dr. Peter HAUSER (NCSU)
Prof. Dr. Oya ATICI (İTÜ) Prof. Dr. Cevza CANDAN (İTÜ) Assoc. Prof. Dr. Mehmet KANIK (UÜ)
BURUŞMAZLIĞIN GELİŞTİRİLMESİ İÇİN PAMUKLU KUMAŞLARIN İYONİK ÇAPRAZ BAĞLANMASI
The author would like to express appreciation for assistance provided by a number of individuals and organizations. Dr. Nevin Çiğdem Gürsoy has provided advice and guidance throughout all this research in USA and in Turkey. Dr. Peter Hauser and Dr. Brent Smith have provided advice and guidance throughout the part of this research conducted in USA. Dr. Oya Atıcı and Dr. Cevza Candan provided advice and guidance throughout the part of this study in Turkey. Jeff Krause provided support in the NCSU College of Textiles pilot plant with equipment used for fabric preparation. Jan Pegram provided support in the NCSU College of Textiles physical testing laboratory with equipment used for physical testing of samples. Judy Ellison provided support with durable press fabric preparation with DMDHEU. Birgit Andersen provided support with the CHN analyzer. Erkmen Ercan and Bilge Hatiboğlu provided support with physical testing of samples.
The author would like to thank İstanbul Technical University for the financial support of this research conducted in USA and in Turkey. He would also like to thank the National Textile Center and the NCSU College of Textiles for financial support of this research conducted in USA. Cotton Incorporated provided the fabric for trials. Dow Chemical provided CR-2000 cationic reagent.
April 2009 Umut Kıvanç Şahin
TABLE OF CONTENTS
LIST OF TABLES... x
LIST OF FIGURES... xii
LIST OF SYMBOLS...xvii
1. INTRODUCTION... 1
1.1 Introduction and Aim of Study... 1
2. LITERATURE REVIEW...3
2.1 Cotton Chemistry... 3
2.2 Why does Cotton Wrinkle?... 5
2.3 Anti-Wrinkle Finish of Cotton...6
2.3.1 Durable press finishing of cotton... 6
18.104.22.168 Urea-formaldehyde derivatives... 8
22.214.171.124 Melamine-formaldehyde derivatives...8
126.96.36.199 Methylol derivatives...8
2.3.2 Alternatives to formaldehyde based DP applications... 9
188.8.131.52 Non-formaldehyde DP applications... 9
184.108.40.206 Ionic crosslinking... 9
2.4 Studies on Imparting Cotton an Ionic Character... 10
2.4.1 Studies on cationic agents... 10
2.4.2 Studies on anionic agents... 12
2.4.3 Studies on both cationic and anionic agents... 13
2.5 Carboxymethylation... 13
2.6 Use of Quaternary Compounds in Textile... 13
3. EXPERIMENTAL... 15
3.1 Materials... 15
3.1.2 Chemicals... 15
3.2 Equipment for Preparation... 17
3.2.1 Stirring hot plate...17
3.2.2 pH meter... 17
3.2.3 Padding machine and oven...17
3.3 Testing... 17
3.3.1 CIE whiteness index and dyeability... 17
3.3.2 Titration... 17
3.3.3 Wrinkle recovery angle... 18
3.3.4 Stiffness... 19
3.3.5 Breaking strength, elongation and energy to peak load... 20
3.3.6 Absorbency... 20
3.3.7 Scanning electron microscope (SEM)...20
3.3.9 Smoothness... 21
3.4 Synthesis of Cationic Agents... 21
3.5 Applied Processes... 23 3.5.1 DMDHEU crosslinking...23 3.5.2 Bleaching...23 3.5.3 NaOH treatment... 24 3.5.4 Carboxymethylation... 24 220.127.116.11 Pad-dry-pad-batch... 24 18.104.22.168 Pad-dry-pad-dry... 25 22.214.171.124 Pad-dry-cure... 25 126.96.36.199 Pad-batch... 25 188.8.131.52 Pad-cure...25 3.5.5 Crosslinking... 25
3.5.6 Dyeing with acid and basic dyes... 25
3.6 Experimental Design... 26
3.6.1 Full factorial experimental design...26
3.6.2 Central composite design... 28
4. RESULTS AND DISCUSSION... 31
4.1 Bleaching... 31
4.2 Ionic Crosslinking... 31
4.2.1 Preliminary experiments... 31
184.108.40.206 Preliminary experiments to choose NaOH% used in preparation of the fabric before carboxymethylation... 31
220.127.116.11 Preliminary experiments to choose cationic agent type... 33
18.104.22.168 Preliminary experiments to choose application process of cationic agent... 35
22.214.171.124 Preliminary experiments to choose the final drying...36
126.96.36.199 Preliminary experiments to choose base levels for the experimental design... 36
4.2.2 Results of full factorial designed experiments... 39
188.8.131.52 Carboxymethyl content... 39
184.108.40.206 Nitrogen content... 39
220.127.116.11 WRA... 44
18.104.22.168 Stiffness... 50
22.214.171.124 Smoothness... 60
126.96.36.199 CIE whiteness index and dyeaility... 60
188.8.131.52 Breaking strength, elongation and energy to peak load... 84
4.2.3 Results of central composite designed experiments...111
184.108.40.206 Estimated optimized recipes and estimated response values... 111
220.127.116.11 Actual optimized recipes and their response values...113
4.3 Comparison of the Response Values of Chosen Optimized Recipe Treated Fabric with Those of Traditionally (DMDHEU) Treated Fabric... 113
4.4 Comparison of the Yarn Strength and SEM Images of Selected PDPB Treated Samples with Those of Traditionally (DMDHEU) Treated Fabric... 114
4.5 Reproducibility of Ionic Crosslinking... 120
6. FUTURE WORK... 127
AGU : Anhydro Glucose Unit
ANOVA : Analysis of Variance
BTCA : 1,2,3,4-ButaneTetraCarboxylic Acid
CAA : ChloroAcetic Acid
CC : Cationized Chitosan
CG : Cationic Glycerin
CH4 : Methane
CHN : Carbon Hydrogen Nitrogen
CHTAC : 3-Chloro-2-Hydroxypropyl-Trimethyl Ammonium Chloride
CM : Carboxymethyl
CO : Carbon Monoxide
CO2 : Carbon Dioxide
COO- : Carboxyl
DHDMI : Dihydroxy Dimethyl Imidazolidinone
DMDHEU : Dihydroxyethylene urea-formaldehyde
DMeDHEU : Dimethyl Dihydroxy Ethylene Urea
DP : Durable Press
EDTA : Ethylene Diamine Tetraacetic Acid
EPTAC : EpoxyPropyl Trimeethyl Ammonium Chloride
GTMAC : GlycidylTriMethylAmmonium Chloride
H2O2 : Hydrogen Peroxide
HCl : Hydro Chloric Acid
HEDTA : N-(2-Hydroxyethyl) Ethylene Dinitrilo Triacetic Acid
HS+OD : Hot Soaked and Oven Dried
HS+RT : Hot Soaked and dried at Room Temperature
HTCC : N-(2 Hydroxy) propyl-3-Trimethylammonium Chitosan
L.R. : Liquor Ratio
NaOH : Sodium Hydroxide
NTA : Nitrilo riacetic acid Trisodium salt monohydrate
OT : Optimum Treated
PB : Pad-Batch
PC : Pad-Cure
PCA : PolyCarboxylic Acid
PDC : Pad-Dry-Cure
PDPB : Pad-Dry-Pad-Batch
PDPD : Pad-Dry-Pad-Dry
S+OD : Soaked and Oven Dried
SEM : Scanning Electron Microscope
LIST OF TABLES
Table 3.1: Coded and actual design levels for full factorial experimental design... 26
Table 3.2: Full factorial experimental design of the study... 27
Table 3.3: Central composite design in coded level... 29
Table 3.4: Central composite design in actual level... 30
Table 4.1: Carboxymethylation levels of samples treated by using different levels of NaOH prior to treatment with 1M Na salt of CAA + 3% CG... 32
Table 4.2: WRA results for various alcohol groups of cationic agent... 34
Table 4.3: Breaking strength, elongation, energy to peak load and stiffness results for various alcohol groups of cationic agent... 35
Table 4.4: Effect of hot soaking and drying processes on WRA... 35
Table 4.5: Effect of drying method on WRA...36
Table 4.6: Titration results for five different carboxymethylation procedures... 36
Table 4.7: WRA results for five different carboxylethylation procedures... 37
Table 4.8: Breaking strength results for five different carboxymethylation procedures... 37
Table 4.9: Titration and WRA results for various pad-batch trials... 38
Table 4.10: Carboxymethyl contents of anionic cotton samples (mmole/100g cotton)... 39
Table 4.11: Coded ID and average nitrogen content values... 40
Table 4.12: Prob > F values for nitrogen content responses of PDPD, PDPB and PDC trials... 43
Table 4.13: Coded ID and average WRA values... 44
Table 4.14: Prob > F values for dry and wet WRA responses of PDPD, PDPB and PDC trials... 49
Table 4.15: Coded ID and stiffness values in warp and filling directions for ionic crosslinked samples...50
Table 4.16: Prob > F values for stiffness in warp direction and stiffness in filling direction responses of PDPD, PDPB and PDC trials... 56
Table 4.17: Coded ID and smoothness values for ionic crosslinked samples... 60
Table 4.18: Prob > F values for smoothness responses of PDPD, PDPB and PDC trials... 64
Table 4.19: Coded ID, CIE whiteness index values for ionic crosslinked samples and L*, C*, h* values for samples dyed with acid dye... 65
Table 4.20: Coded ID and L*, C*, h* values for samples dyed with basic dye... 67
Table 4.21: Prob > F values for CIE whiteness index and L*, C* and h* responses of PDPD, PDPB and PDC trials... 68
Table 4.22: Coded ID, average breaking strength, elongation and energy to peak load values of ionic crosslinked samples in warp direction... 84
Table 4.23: Coded ID, average breaking strength, elongation and energy to peak load values of ionic crosslinked samples in filling direction... 86
Table 4.24: Prob > F values for breaking strength, elongation and energy to
peak load responses of PDPD, PDPB and PDC trials...88
Table 4.25: Coded and actual design factor levels for optimization... 111 Table 4.26: Estimated response values for optimum PDPB recipes... 112 Table 4.27: Prob > F values for dry and wet WRA responses of optimization
Table 4.28: Actual chemical and response values for optimum PDPB recipes... 113 Table 4.29: Breaking strength, elongation, energy to peak load and CIE whiteness
index values for untreated, DMDHEU treated and OT samples... 113
Table 4.30: Tensile strength values for untreated, DMDHEU treated and
selected ionic crosslinked yarn samples... 114
Table 4.31: CM contents (mmoles/100g cotton) for 10 fabrics... 121 Table 4.32: WRA, CM, nitrogen content and stiffness values for 10 fabrics... 121 Table 4.33: Average breaking strength, elongation and energy to peak load
results for 10 fabrics in warp direction... 122
Table 4.34: Average breaking strength, elongation and energy to peak load
results for 10 fabrics in filling direction... 122
Table 4.35: CIE whiteness index, L*, C*, h* and nitrogen content results for
10 fabrics after coloration with acid dye... 123
Table 4.36: CIE whiteness index, L*, C*, h* and nitrogen content results for
LIST OF FIGURES
Figure 2.1 : Molecular structure of a cellulose polymer chain. ... 3
Figure 2.2 : Formation of wrinkle . ... 6
Figure 2.3 : Reaction scheme of a typical crosslinking process ... 7
Figure 3.1 : Synthesis of cationic glycerin. ... 22
Figure 3.2 : Bleaching procedure. ... 24
Figure 3.3 : Dyeing procedure. ... 26
Figure 4.1 : Second order polynomial fit for NaOH% vs. CM content... 32
Figure 4.2 : Third order polynomial fit for NaOH% vs. CM content. ... 33
Figure 4.3 : Fourth order polynomial fit for NaOH% vs. total WRA. ... 33
Figure 4.4 : The effects of Na salt of CAA and CG on nitrogen content for PDPD treated samples. ... 42
Figure 4.5 : The effects of Na salt of CAA and CG on nitrogen content for PDPB treated samples... 42
Figure 4.6 : The effects of Na salt of CAA and CG on nitrogen content for PDC treated samples... 43
Figure 4.7 : The effects of Na salt of CAA and CG on dry WRA for PDPD treated samples. ... 46
Figure 4.8 : The effects of Na salt of CAA and CG on wet WRA for PDPD treated samples. ... 46
Figure 4.9 : The effects of Na salt of CAA and CG on dry WRA for PDC treated samples. ... 47
Figure 4.10 : The effects of Na salt of CAA and CG on wet WRA for PDC treated samples. ... 47
Figure 4.11 : The effects of Na salt of CAA and CG on dry WRA for PDPB treated samples. ... 48
Figure 4.12 : The effects of Na salt of CAA and CG on wet WRA for PDPB treated samples. ... 48
Figure 4.13 : The effects of Na salt of CAA and CG on stiffness in warp direction for PDPD treated samples. ... 52
Figure 4.14 : The effects of Na salt of CAA and CG on stiffness in warp direction for PDPB treated samples. ... 53
Figure 4.15 : The effects of Na salt of CAA and CG on stiffness in warp direction for PDC treated samples. ... 54
Figure 4.16 : The effects of Na salt of CAA and CG on stiffness in filling direction for PDPD treated samples. ... 54
Figure 4.17 : The effects of Na salt of CAA and CG on stiffness in filling direction for PDPB treated samples. ... 55
Figure 4.18 : The effects of Na salt of CAA and CG on stiffness in filling direction for PDC treated samples. ... 55
Figure 4.19 : Interaction between Na salt of CAA and stiffness in warp direction. ... 56
Figure 4.20 : Interaction between Na salt of CAA and stiffness in filling
Figure 4.21 : Interaction between dry WRA and stiffness in warp direction...57
Figure 4.22 : Interaction between dry WRA and stiffness in filling direction. ...58
Figure 4.23 : Interaction between wet WRA and stiffness in warp direction. ...58
Figure 4.24 : Interaction between wet WRA and stiffness in filling direction. ...59
Figure 4.25 : Interaction between total WRA and stiffness in warp direction...59
Figure 4.26 : Interaction between total WRA and stiffness in filling direction. ...60
Figure 4.27 : The effects of Na salt of CAA and CG on smoothness for PDPD treated samples...62
Figure 4.28 : The effects of Na salt of CAA and CG on smoothness for PDPB treated samples...63
Figure 4.29 : The effects of Na salt of CAA and CG on smoothness for PDC treated samples...63
Figure 4.30 : The effects of Na salt of CAA and CG on CIE whiteness index for PDPD treated samples...69
Figure 4.31 : The effects of Na salt of CAA and CG on CIE whiteness index for PDPB treated samples...69
Figure 4.32 : The effects of Na salt of CAA and CG on CIE whiteness index for PDC treated samples. ...70
Figure 4.33 : Interaction between wet WRA and CIE whiteness index. ...71
Figure 4.34 : Interaction between total WRA and CIE whiteness index. ...71
Figure 4.35 : The effects of Na salt of CAA and CG on L* for PDPD treated and acid dyed samples. ...72
Figure 4.36 : The effects of Na salt of CAA and CG on L* for PDPB treated and acid dyed samples. ...72
Figure 4.37 : The effects of Na salt of CAA and CG on L* for PDC treated and acid dyed samples. ...73
Figure 4.38 : Interaction between Na salt of CAA and L* for samples dyed with an acid dye. ...74
Figure 4.39 : The effects of Na salt of CAA and CG on C* for PDPD treated and acid dyed samples. ...74
Figure 4.40 : The effects of Na salt of CAA and CG on C* for PDPB treated and acid dyed samples. ...75
Figure 4.41 : The effects of Na salt of CAA and CG on C* for PDC treated and acid dyed samples. ...75
Figure 4.42 : The effects of Na salt of CAA and CG on h* for PDPD treated and acid dyed samples. ...76
Figure 4.43 : The effects of Na salt of CAA and CG on h* for PDPB treated and acid dyed samples. ...76
Figure 4.44 : The effects of Na salt of CAA and CG on h* for PDC treated and acid dyed samples. ...77
Figure 4.45 : Interaction between Na salt of CAA and C* for samples dyed with an acid dye...77
Figure 4.46 : Interaction between Na salt of CAA and h* for samples dyed with an acid dye...78
Figure 4.47 : The effects of Na salt of CAA and CG on L* for PDPD treated and basic dyed samples...79
Figure 4.48 : The effects of Na salt of CAA and CG on L* for PDPB treated and basic dyed samples...79
Figure 4.49 : The effects of Na salt of CAA and CG on L* for PDC treated
and basic dyed samples. ... 80
Figure 4.50 : Interaction between Na salt of CAA and L* for samples dyed
with a basic dye... 80
Figure 4.51 : The effects of Na salt of CAA and CG on C* for PDPD treated
and basic dyed samples. ... 81
Figure 4.52 : The effects of Na salt of CAA and CG on C* for PDPB treated
and basic dyed samples. ... 81
Figure 4.53 : The effects of Na salt of CAA and CG on C* for PDC treated
and basic dyed samples. ... 82
Figure 4.54 : The effects of Na salt of CAA and CG on h* for PDPD treated
and basic dyed samples. ... 82
Figure 4.55 : The effects of Na salt of CAA and CG on h* for PDPB treated
and basic dyed samples. ... 83
Figure 4.56 : The effects of Na salt of CAA and CG on h* for PDC treated
and basic dyed samples. ... 83
Figure 4.57 : The effects of Na salt of CAA and CG on breaking strength
in warp direction for PDPD treated samples. ... 89
Figure 4.58 : The effects of Na salt of CAA and CG on breaking strength
in warp direction for PDPB treated samples... 89
Figure 4.59 : The effects of Na salt of CAA and CG on breaking strength
in warp direction for PDC treated samples... 90
Figure 4.60 : The effects of Na salt of CAA and CG on breaking strength
in filling direction for PDPD treated samples... 90
Figure 4.61 : The effects of Na salt of CAA and CG on breaking strength
in filling direction for PDPB treated samples. ... 91
Figure 4.62 : The effects of Na salt of CAA and CG on breaking strength
in filling direction for PDC treated samples... 92
Figure 4.63 : The effects of Na salt of CAA and CG on elongation in warp
direction for PDPD treated samples. ... 92
Figure 4.64 : The effects of Na salt of CAA and CG on elongation in warp
direction for PDPB treated samples. ... 93
Figure 4.65 : The effects of Na salt of CAA and CG on elongation in warp
direction for PDC treated samples. ... 93
Figure 4.66 : The effects of Na salt of CAA and CG on elongation in filling
direction for PDPD treated samples. ... 94
Figure 4.67 : The effects of Na Salt of CAA and CG on elongation in filling
direction for PDPB treated samples. ... 94
Figure 4.68 : The effects of Na salt of CAA and CG on elongation in filling
direction for PDC treated samples. ... 95
Figure 4.69 : The effects of Na salt of CAA and CG on energy to peak load
in warp direction for PDPD treated samples. ... 96
Figure 4.70 : The effects of Na salt of CAA and CG on energy to peak load
in warp direction for PDPB treated samples. ... 96
Figure 4.71 : The effects of Na salt of CAA and CG on energy to peak load
in warp direction for PDC treated samples. ... 97
Figure 4.72 : The effects of Na salt of CAA and CG on energy to peak load
in filling direction for PDPD treated samples. ... 98
Figure 4.73 : The effects of Na salt of CAA and CG on energy to peak load
Figure 4.74 : The effects of Na salt of CAA and CG on energy to peak load
in filling direction for PDC treated samples. ...99
Figure 4.75 : Interaction between Na salt of CAA and breaking strength
in warp direction. ...99
Figure 4.76 : Interaction between Na salt of CAA and elongation in warp
Figure 4.77 : Interaction between Na salt of CAA and energy to peak load
in warp direction. ...100
Figure 4.78 : Interaction between Na salt of CAA and breaking strength
in filling direction...101
Figure 4.79 : Interaction between Na salt of CAA and elongation in filling
Figure 4.80 : Interaction between Na salt of CAA and energy to peak load
in filling direction...102
Figure 4.81 : Interaction between dry WRA and breaking strength in warp
Figure 4.82 : Interaction between dry WRA and elongation in warp direction. ....103 Figure 4.83 : Interaction between dry WRA and energy to peak load in warp
Figure 4.84 : Interaction between dry WRA and breaking strength in filling
Figure 4.85 : Interaction between dry WRA and elongation in filling
Figure 4.86 : Interaction between dry WRA and energy to peak load in filling
Figure 4.87 : Interaction between wet WRA and breaking strength in warp
Figure 4.88 : Interaction between wet WRA and elongation in warp direction...106 Figure 4.89 : Interaction between wet WRA and energy to peak load in warp
Figure 4.90 : Interaction between wet WRA and breaking strength in filling
Figure 4.91 : Interaction between wet WRA and elongation in filling
Figure 4.92 : Interaction between wet WRA and energy to peak load in filling
Figure 4.93 : Interaction between total WRA and breaking strength in warp
Figure 4.94 : Interaction between total WRA and elongation in warp
Figure 4.95 : Interaction between total WRA and energy to peak load in warp
Figure 4.96 : Interaction between total WRA and breaking strength in filling
Figure 4.97 : Interaction between total WRA and elongation in filling
Figure 4.98 : Interaction between total WRA and energy to peak load in
Figure 4.99 : Tensile breaks of raw cotton...115 Figure 4.100 : Tensile breaks of resin treated cotton...115
Figure 4.101 : Tensile break of bleached cotton. ... 116
Figure 4.102 : Tensile breaks of DMDHEU treated cotton... 117
Figure 4.103 : Tensile break of sample 231... 118
Figure 4.104 : Tensile break of sample 233... 118
Figure 4.105 : Tensile break of sample 235... 119
Figure 4.106 : Tensile break of sample 251... 119
Figure 4.107 : Tensile Break of sample 253. ... 119
LIST OF SYMBOLS
C* : Chroma value according to CIELAB Color Scale h* : Hue value according to CIELAB Color Scale L* : Lightness value according to CIELAB Color Scale NHCl : Normality of HCl used
Vblank : Volume of titrant used for blank Vsample : Volume of titrant used for sample Vtitrant : Volume of titrant used
W,w : Weight
IONIC CROSSLINKING OF COTTON FABRICS TO IMPROVE WRINKLE RECOVERY
Cotton fiber has a natural tendency to wrinkle. In order to overcome this undesired property of cotton several durable press finishes were proposed and have been used for a long while. However, most of these chemical finishes release formaldehyde, a suspected human carcinogen, and cause fabric to lose strength and to yellow. Non-formaldehyde alternatives to these finishes are expensive. Thus, a non-Non-formaldehyde finish prepared by using common and more available chemicals is required. In this study, we prepared anionic cotton fabric by following 3 different carboxymethylation methods and further treated it with a novel crosslinker, namely cationic glycerin. We focused on optimizing ionic crosslinking process in terms of treated fabric’s wrinkle recovery angle (WRA). We also tested our samples for strength, elongation, stiffness, smoothness, whiteness and nitrogen content. In order to investigate the effect of ionic crosslinking on dyeability, we dyed our treated samples with an acid and a basic dye. Our results showed that high WRA results may be achieved and strength of fabric may also be increased by ionic crosslinking. After ionic crosslinking treatment, elongation of cotton fabric was increased. Stiffness and smoothness of cotton fabric increased but to a limited extent. Dyeability of cotton with basic dyestuff got better as well. These results show that ionic crosslinking is a good alternative to conventional durable press finishes.
PAMUKLU KUMAŞLARIN BURUŞMAZLIK ÖZELLİKLERİNİN GELİŞTİRİLMESİ İÇİN İYONİK ÇAPRAZ BAĞLANMALARI ÖZET
Pamuk lifinin buruşmaya karşı doğal bir eğilimi vardır. Pamuğun bu istenmeyen özelliğini gidermek için uzun süredir pek çok kalıcı ütü apreleri önerilmektedir ve kullanılmaktadır. Ancak, bu kimyasal aprelerin çoğu, kanser yapma ihtimali olduğundan şüphelenilen formaldehiti açığa çıkarırlar ve kumaşın mukavemet kaybetmesine ve sararmasına sebep olurlar. Bu aprelere alternatif olan formaldehitsiz kimyasallar pahalıdırlar. Bu nedenle, yaygın ve kolay ulaşılabilir kimyasallar kullanılarak hazırlanan bir formaldehitsiz apreye ihtiyaç vardır. Bu çalışmada, 3 farklı karboksimetilasyon yöntemi kullanarak anyonik pamuklu kumaş hazırladık ve daha sonra bunu katyonik gliserin adı verilen yeni bir çapraz bağlayıcı ile muamele ettik. Muamele edilen kumaşın buruşmazlık açısına göre iyonik çapraz bağlama işlemini optimize etmeye odaklandık. Numunelerimizi ayrıca mukavemet, uzama, sertlik, düzgünlük, beyazlık ve nitrojen miktarı için de test ettik. İyonik çapraz
bağlamanın boyanabilirliğe etkisini incelemek için muamele ettiğimiz
numunelerimizi bir asidik bir de bazik boya ile boyadık. Sonuçlarımız göstermektedir ki iyonik çapraz bağlama ile yüksek buruşmazlık açısı değerleri elde edilebilmektedir ve kumaş mukavemeti de artırılabilmektedir. İyonik çapraz bağlama muamelesinden sonra pamuklu kumaşın uzaması artmıştır. Pamuklu kumaşın sertliği ve düzgünlüğü artmıştır fakat bu sınırlı bir seviyededir. Ayrıca pamuğun bazik boyarmadde ile boyanabilirliği de artırılmıştır. Bu sonuçlara göstermektedir ki iyonik çapraz bağlama konvansiyonel kalıcı ütü aprelerine iyi bir alternatiftir.
1.1 Introduction and Aim of Study
In this study, our aim was to show that ionic crosslinking could be a good alternative to conventional durable press finishing. We followed a designed experiment and optimized the ionic crosslinking process in terms of resulting fabric’s wrinkle recovery angle (WRA). In previous studies, treating anionic cotton with cationic agents were shown to impart the highest WRA values on cotton fabric when ionic crosslinking was followed, but only one carboxymethylation method was used in these previous studies, a pad-dry-pad-batch (PDPB) method [1-3]. In our trials we used this method and two other alternative carboxymethylation processes, and investigated their effects on resulting WRA in an effort to decrease process time. One of these methods is pad-dry-pad-dry (PDPD) which is a shorter procedure. The other is pad-dry-cure (PDC) method, which is the shortest one but requires a high temperature step. We used cationic glycerin in our entire crosslinking trials. Cationic glycerin and cationic chitosan are the cationic agents that impart the highest WRA results but cationic glycerin has a lot of advantages when compared with cationic chitosan; it offers better breaking strength, whiteness and stiffness values . It is also cheaper and more available. We also investigated the effects of ionic crosslinking on strength, elongation, stiffness, smoothness, whiteness, nitrogen content and dyeability with acid and basic dyes.
2. LITERATURE REVIEW
2.1 Cotton Chemistry
Cotton fibers are the purest form of cellulose which is the most abundant polymer in the nature. Almost 90% of the cotton fibers are cellulose. The cellulose in cotton fibers has the highest molecular weight among all plant fibers and the highest structural order, i.e., highly crystalline, oriented and fibrillar .
Cotton fibers are composed of mostly α-cellulose (88.0-96.5%). The noncellulosics are located either on the outer layers (cuticle and primary cell wall) or inside the lumens of the fibers whereas secondary cell wall is purely cellulose. The varieties of these are affected by growing environments (soil, water, temperature, pest, etc.) and maturity. The noncellulosics include proteins (1.3%), waxes (0.6%), pectins (1.2%), ash (1.2%), and other (1.7%) substances. In less developed or immature fibers, the non-cellulosic contents are much higher than the mature ones [4,5].
Figure 2.1 :Molecular structure of a cellulose polymer chain.
Cotton cellulose is highly crystalline and oriented. α-cellulose is distinct in its long and rigid molecular structure. The β-1,4-D(+)-glucopyranose building blocks in long cellulose chains are linked by 1,4-glucosidic bonds (see Figure 2.1). Free formation of the anhydrogluco-pyranose C-O-C link is prevented by steric effects. Each anhydroglucose contains three hydroxyl groups, one primary on C-6 and two secondary on C-2 and C-3. The abundant hydroxyl groups and the chain conformation allow extensive inter-molecular and intra-molecular hydrogen bonding to further improve the rigidity of the cellulose structure [4,6].
Effects of chemical reactions and heating on cellulose depends on the supermolecular structure and the activity of the C-2, C-3 and C-6 hydroxyl groups. Heat or reactions begin in the more accessible amorphous regions and the surfaces of crystalline domains. Chemical reactivity of the cellulose hydroxyl groups follows those of aliphatic hydroxyl groups, i.e., higher for the C-6 primary than the secondary on the C-2 and C-3. Etherification and esterification are the two main categories of reaction. Esterification reactions, such as nitration, acetylation, phosporylation, and sulfation, are usually carried out under acidic conditions. Etherification, on the other hand, is favored in an alkaline medium .
Oxidizing agents, such as hypochlorites, chlorus, chloric, and perchloric acids, peroxides, dichromates, permanganates, periodic acid, periodate salts, and nitrogen tetroxide readily attack cellulose. Most of these agents are not selective in the way they react with the primary and secondary hydroxyl groups. Oxidation of cellulose can result in two products, reducing and acidic oxycellulose. In reducing oxycellulose, the hydroxyl groups are converted to carbonyl groups or aldehydes, whereas in acidic oxycellulose, the hydroxyl groups are oxidized to carbonyl groups or acids. The oxycellulose can be further oxidized to acidic oxycellulose. Reducing oxycellulose is more sensitive to alkaline media and the chain lengths are often reduced. Periodic acid and periodate salts break the anhydroglucose ring between C-2 and C-3, converting the two secondary hydroxyl to aldehydes which can be further oxidized to carboxyl groups. Nitrogen tetroxide reacts specifically with the primary hydroxyl groups on C-6 and directly oxidizes it to carboxyl group or to polyglucuronic acid, an oxycellulose [4,6].
Dehydration and decomposition of cellulose are the general results of heating of cellulose. Presence of other compounds, the temperature and rate of heating affects these reactions. Presence of acid catalysts favor dehydration reactions whereas depolymerization reactions are favored by alkaline catalysts. Dehydration is favored by heating at low temperatures and subsequent char formation is enhanced. Higher temperature heating causes rapid volatilization via the formation of laevoglucosan and more gaseous combustible products are formed. Greater dehydration also reduces the yield of laevoglucosan and subsequently lowers the volatile species. For that reason, acid catalysts are especially important in order to impart flame retardancy to cellulose [4,5].
When cellulose is heated up to 120oC, the moisture is driven off without affecting strength. Heating cellulose to 150oC reduce viscosity and tensile strength which show that molecular weight is lowered. Between 200oC and 300oC, volatile products and liquid pyrolyzate, mainly 1,6-anhydro-β-D-glucopyranose, commonly known as levoglucosan, evolve. At 450°C, only char remains. 20% of total pyrolytic products is gaseous phase (CO, CO2, and CH4), 65% of them is the liquid phase (of which
80% is levoglucosan) and 15% of them is the char. The heating rate can influence the amount of char formation. Heating below 250°C only influences amorphous regions as no change in the crystalline structure has been found. The crystalline structure of cellulose has been shown to be lower when heated at 250oC to 270oC, and then disappear on further heating to 300oC. Highly crystalline cellulose has been shown to decompose at higher temperatures, for instance 380oC [4-6].
Depolymerization is prevented by blocking the primary hydroxyl groups of cellulose and production of volatiles are reduced as well. The reduction of flammable gases is accompanied by more complete intra-ring and inter-ring dehydration, giving rise to keto-enol tautomers and ethermic linkages, respectively. The carbonyl groups so formed can participate in a variety of reactions, leading to crosslinking, thus increasing char formation as well as carbon dioxide. The packing density of cellulose also affects the extent of levoglucosan formation. Higher yield of levoglucosan formation is reached when crystallinity in cotton is lowered by either mercerization or liquid ammonia. Cleavage of glucoside linkages form mono- and difunctional radicals. These radicals increases volatile products and levoglucosan .
2.2 Why does Cotton Wrinkle?
Wrinkles occur when fabrics are crushed during use and care like washing. Wrinkle recovery depends on crosslinks, which hold adjacent molecular chains together and pull them back into position after the fiber is bent, thus preventing the formation of a wrinkle. Fibers with strong intermolecular bonds have good molecular memory and resist wrinkling and creasing. Fibers with weak bonds wrinkle and crease readily. Cellulosic fibers lack strong natural crosslinks. Their molecular chains are held together by weak hydrogen bonds and these bonds break with the stress of bending particularly when the fiber is wet. New hydrogen bonds are formed; they hold the
Figure 2.2 : Formation of wrinkle . 2.3 Anti-Wrinkle Finish of Cotton
2.3.1 Durable press finishing of cotton
Durable press finishes are an important treatment for cotton fabrics; they provide wrinkle resistant and permanent press performance for apparel. The cellulose chains are covalently bond together by crosslinking and these covalent bonds cannot be disrupted by water. The reaction steps of a typical crosslinking process are schematically shown in Figure 2.3. A dry fabric is impregnated with a mixture of crosslinking agents and reaction auxiliaries by means of a foulard. The fabric is mildly dried and then cured on special machines. The pre-polymers crosslink to form long chains of resin or link to the fiber surface. Initiation of condensation requires addition of acid and the reaction temperature has to be high .
Crosslinking processes may be classified into 2 groups according to the state of the fabric just before the reaction. First one of these is dry crosslinking process that is by far the most applied process. In dry crosslinking; a dry fabric is impregnated with a mixture of the polymer resin, auxiliaries and catalysts. It is then dried and cured to enable the condensation of the resins.
Second one is wet or moist crosslinking process, in which the cellulose fibers of the already wet fabric are swelled. The crosslinking agent is impregnated into the fabric in strong alkali or mineral acid medium. The overall product is left for nearly 24 hours in order to permit crosslinking. The effects of these 2 methods are quite different. The dry crosslinking reactions impart good constancy when wrinkled in the dry state but their stability is moderate after wetting. On the contrary, resin-free
crosslinking improves the wet wrinkle resistance, but the fabric tends to crease when dry .
Figure 2.3 : Reaction scheme of a typical crosslinking process .
There are two types of products used in conventional durable press finishing; resin type and reactant type. Resin type products are the firstly commercialized ones.
18.104.22.168 Urea-formaldehyde derivatives
Use of amino resin finishing for the production of crease-resistant fabrics commenced in 1920s with the manufacture of simple urea-formaldehyde resins. After urea, a full range of products was developed. All of these products contain formaldehyde, such as urea-formaldehyde, highly condensated urea-formaldehyde, methylated urea-formaldehyde, formaldehyde, methylated melamine-formaldehyde, ethylene urea-melamine-formaldehyde, heterocyclic crosslinking agents based on melamine-formaldehyde, glycol based reactants and their derivatives. Urea-formaldehyde resins were very popular in 1940s. However, the fabric required washing off due to high free formaldehyde content of the resin. In 1950s methylated urea-formaldehyde resins came onto the market. They were applicable on nylon and when compared with urea-formaldehyde resins they had greater durability to washing, better shrink-stability of the treated fabric, and stability of the molecular size. Producing a stiff handle on synthetic fibers and giving high formaldehyde contents were some of the negative properties of urea-formaldehyde resins .
22.214.171.124 Melamine-formaldehyde derivatives
The next resin group commercialized was melamine resins. Among these, trimethylol melamins were the most popular ones. When compared with urea-formaldehyde resins, they give a fuller handle on cotton and viscose, but they were more expensive .
126.96.36.199 Methylol derivatives
To overcome the disadvantages of resin type products, reactant-type products were produced and they came in the market in the early 1960s. As a result of reacting only with the cellulose component, these products offered softer handle of blended fabrics. They had lower formaldehyde content, and required smaller amounts of resin to produce comparable results with resin formers. Unlike older resins that form a polymeric network within the fiber, reactant products actually react with the fiber. Some examples of reactant-type products are ethylene urea-formaldehyde, propylene formaldehyde, methylated uron-formaldehyde and dihydroxyethylene urea-formaldehyde (DMDHEU). The most popular reactant-type product is the DMDHEU type and its modifications. DMDHEU resins are produced by a reaction of glyoxal, urea and formaldehyde. The low-formaldehyde versions of DMDHEU are widely
used. These have been modified to produce a low-formaldehyde resin by using diethylene glycol as a formaldehyde acceptor. The formaldehyde figure can be reduced by approximately 50%, compared with the original DMDHEU resin .
2.3.2 Alternatives to formaldehyde based DP applications 188.8.131.52 Non-formaldehyde DP applications
Durable press finishes free of formaldehyde or formaldehyde precursors have also been proposed. Some of these are dimethyl dihydroxy ethylene urea (DMeDHEU), dihydroxy dimethyl imidazolidinone (DHDMI), polycarboxylic acids such as citric acid and butane tetracarboxylic acid, with hyposphosphite salts, imidazoles or sodium maleate, sodium tartrate or sodium citrate as catalysts and citric acid as extender. Other systems based on polyacrylics, polyurethane and silicones are also offered. Reactive polymeric silicones appear to be interesting as they impart simultaneously non-creasing, waterproof, soil-release properties. These zero-formaldehyde finishing systems do not appear to compete with DMDHEU-type products because of their higher cost. By adding suitable additives such as polyhydric alcohols, phosphorous catalysts or sodium salt of hydroxyl acids, the cost of these finishing systems may be reduced. However, the molecular weight and thus the strength of the fabric decreases, yellowing of the fabric increases and the finish is less durable [8, 10].
184.108.40.206 Ionic crosslinking
It is apparent that a non-formaldehyde finish prepared by using common and more available chemicals is required. For this purpose researchers have been recently working on using ionic crosslinking as an alternative mechanism for producing durable press performance. Hashem, Hauser and Smith offered an ionic crosslinking process, in which an ionic site is imparted to cotton and then it is crosslinked by using a polyion of the opposite charge [1, 2]. In his study , Bilgen reacted cellulose with sodium salt of chloroacetic acid (CAA) and then crosslinked it with cationic chitosan, cationic glycerin (CG), calcium chloride, magnesium chloride, cationized ethylene glycol, cationized dextrose, cationized D-celobiose and cationized ß-cyclodextrin. He also reacted cellulose with 3-chloro-2-hydroxypropyl-trimethyl ammonium chloride (CHTAC) and crosslinked it with polycarboxylic acid
(PCA), 1,2,3,4-butanetetracarboxylic acid (BTCA), ethylene diamine tetraacetic acid (EDTA), nitriloriacetic acid trisodium salt monohydrate (NTA), N-(2-hydroxyethyl) ethylene dinitrilotriacetic acid (HEDTA), oxalic acid, citric acid and maleic acid. All of these crosslinking agents demonstrated improvement in wrinkle resistance but the higher WRA results are gained when carboxymethylated (anionic) cotton is reacted with cationic agents synthesized by reaction of a quaternary compound, namely 3-chloro-2-hydroxypropyl-trimethyl ammonium chloride (CHTAC), with chitosan or glycerin. There is no formaldehyde release or strength loss unlike conventional methods and WRA results for such treated cotton fabric are promising but yet an optimized procedure for ionic crosslinking is still needed.
2.4 Studies on Imparting Cotton an Ionic Character
Many studies have been made on cationic and anionic agents to be used in imparting cotton an ionic character, some of which are briefly reviewed below.
2.4.1 Studies on cationic agents
Rupin studied on reactive and direct dyeing of cotton, which was aminated by an epoxy quaternary ammonium compound, namely glycidyl trimethyl ammonium chloride. He listed some advantages of amination as; not needing a fixing agent in dyeing because of the ionic bond formed, savings of rinse water and wastewater treatment, and savings in the amount of the dye needed. He added that the cost due to addition of necessary nitrogen content could be balanced with these savings . Ungeful and Sello used divalent cations to form ionic crosslinks that increased the strength properties of the acrylic polymer film used in acrylic sizes. They increased the tensile strength of these copolymer films while reducing their moisture sensitivity .
Evans, Shore and Stead studied on reactive quaternary agents used to modify cotton. They compared epoxypropyl type agents with chlorotriazine ones, and gave detailed information on preparation and evaluation of chlorotriazine-type quaternary agents .
Lewis and Lei made a literature review about modifying cellulose by reactive compounds to covalently bind secondary amino, tertiary amino, quaternary amino,
thiol or disulfide residues. Some of those chemicals were 2-aminoethylsulfate, glycidil-trimethyl ammonium chloride (or its precursor 1-trimethyl-ammonium-2-hydroxy-3-chloropropane chloride), β-chloroethyl-diethylamino hydrochloride, and 2,4-difluoromonochloropyrimidine. They suggested that as a result of increased cellulose hydroxyl ionization due to the proximity of strong basic groups, the neutral fixation was improved in chemicals that introduce tertiary and quaternary amino groups .
Wu and Chen pretreated cotton by using polyepichlorohydrin-dimethylamine to investigate its dyeability properties with reactive dyes. They stated that dyeability of cotton was increased by introducing amino groups, and added that only one tenth of normal amount of salt was needed when exhaust dyeing such treated cotton under neutral condition with low-reactivity dyes and no salt was needed with high-reactivity dyes .
Kim, Choi and Yoon synthesized a quaternary ammonium derivative of chitosan, namely N-(2 hydroxy) propyl-3-trimethylammonium chitosan (HTCC), to be used as an antimicrobial finish, by reacting chitosan with glycidyltrimethylammonium chloride (GTMAC). They gave details on the reaction of GTMAC with chitosan to give HTCC (Reaction occurred between GTMAC and NH2 groups in chitosan). They
investigated the antimicrobial activity of cotton fabrics treated with HTCC, and the laundering durability of HTCC .
Kamel, Youssef and Shokry studied the dyeing conditions and dyeing properties of cationized cotton using dimethyl-3-hydroxy-azetidinium chloride and 1,1-diethyl-3-hydroxy-azetidinium chloride .
Kanik and Hauser investigated the effect of cationic pretreatment on reactive printing of cotton. They treated cotton with aqueous solution of N-(3-chloro-2-hydroxypropyl) trimethyl ammonium chloride in the presence of alkali (sodium hydroxide) and printed it with different pastes. They concluded that color yield of the prints was increased especially with medium dye concentrations, steaming time was reduced and washing-off procedure was shortened .
Hauser gave a detailed background of conventional dyeing procedures and reactions of cationic reactant 2,3-epoxypropyltrimethylammonium chloride. He compared commercial dyeing procedures for conventional and cationic cotton .
Hauser and Tabba studied on improving the affinity of anionic dyes for cotton by adding cationic dye sites to this fiber. They used 2,3 epoxypropyl trimethylammonium chloride for the modification of cotton, and they dyed modified cotton using direct, reactive and acid dyes. They concluded that cotton treated with such a reactant gives excellent color yields and color fastness values with direct and reactive dyes without the need for the electrolyte in the dyebath. They added that dyeing procedures for cationic cotton are shorter, use less water and chemical auxiliaries, and require less energy. They concluded that dyeings with acid dyes resulted in darker shades when compared to acidic dyeings of untreated cotton . Hauser and Tabba studied on cationized cotton and applied a salt and non-afterscour dyeing procedure. They used 2,3 epoxypropyl trimethylammonium chloride to impart a cationic charge on cotton fibers. They basically used 3 different reactive dyeing procedures, and reached equivalent fastness values with higher color yields with cationic cotton when compared with fabrics dyed according to supplier recommendations .
Hashem, Refaie and Habeish investigated the effects of NaOH concentration, reaction time and temperature, quaternizing agent concentration, material to liquor ratio and method used for quaternization on quaternization reaction of partially carboxymethylated cotton fabric with 3-chloro-2-hydroxypropyl trimethyl ammonium chloride. They concluded that ionic crosslinking of cotton fabric significantly improved its wet crease recovery angle, tensile strength, and elongation at break with a little improvement in dry recovery angle compared with that of untreated cotton fabric. They also concluded that cold pad-batch method yielded higher N% and fixation % results than those obtained with exhaustion method .
2.4.2 Studies on anionic agents
Kim, Yoon and Son synthesized an anionic agent containing a dichloro-s-triazinyl reactive group by a 3-step reaction, and treated this chemical on cotton fibers to be able color cotton fibers with cationic Berberine colorant. They found that the exhaustion of Berberine to the cotton fibers was 23 times higher than that of the untreated sample and 10 times higher than that of tannic acid pretreated samples .
2.4.3 Studies on both cationic and anionic agents
Hashem, Hauser and Smith studied on synthesis and application on cotton of a cationized chitosan (CC). CC was synthesized in alkaline conditions and the substitution was made on the hydroxyl sites. Furthermore, they offered 5 different methods for ionic crosslinking cellulosic fabric, and applied two of those. They concluded that crease angle recovery was imparted on cotton fabric by ionic crosslinking, generally with strength gain .
Hashem, Hauser and Smith investigated the reaction efficiency for cellulose cationization using CHTAC and concluded that fixation of CHTAC on cellulosic fabrics varied greatly with the choice of method, CHTAC concentration used, alkali amount, time, temperature, and other parameters of the method .
The primary aim of wet processing of textile materials is to increase their usefulness and added values while preserving their natural properties. One of these widely used processes is called carboxymethylation in which carboxyl (COO-) groups are attached to the primary alcohol of anhydroglucose unit.
The process generally consists of treating the material with solutions of monochloroacetic acid and sodium hydroxide. The order of application of these solutions may alternate [24-27] or a mixture of these may be used [28, 29] according to the procedure, always followed by acidification in a dilute aqueous hydrochloric, sulfuric or acetic acid solution. The resulting material is very swellable and has highly acidic carboxyl groups  giving enhancements in water retention, moisture regain, soil release, tensile strength and elongation at break [26, 28, 31]. A very good review of studies on carboxymethylation is given by Racz, Deak and Borsa .
2.6 Use of Quaternary Compounds in Textile
Use of quaternary compounds in modification of cotton for further use in finishing and dyeing started in mid 70s with amination prior to dyeing, which brought savings in fixing agent, rinse water and dye needed . Many researchers worked with cationic agents and reported positive results, some of which are increase in dyeability , decrease in amount of electrolyte needed [15, 20], higher color yield [20, 21],
shorter processing time, less need for water and chemicals and thus energy savings  in dyeing, increased wash fastness and processing speed in printing , and increase in antimicrobial activity . Detailed information on reactions of 2,3 epoxypropyl trimethyl ammonium chloride and comparison of commercial dyeing procedures for conventional and cationic cotton is given by Hauser .
3.1 Materials 3.1.1 Fabric
The fabric used in this study was a 100% standard plain weave cotton fabric (style 400, 44”- 45”, 78 X 76, ISO 105/F02) supplied from Testfabrics Inc. The fabric weight was measured as 102 g/m2. The fabric did not have absorbency for an observation time of 60 seconds.
All solution percentages are expressed as weight on weight. Reagent used for synthesis of the cationic crosslinkers:
• N-(3-chloro-2-hydroxypropyl) trimethylammonium chloride (CHTAC):
69%, CR2000, Dow Chemicals Company
Alcohols used for synthesis of the cationic crosslinkers: • Glycerin: 99%, Fisher Chemicals Company
• Ethylene Glycol: Laboratory grade, Fisher Chemicals Company • Ethyl Alcohol: Denaturated, Fisher Chemicals Company
• 1,2-Propanediol: 99%, Acros Chemical Company • 1,3-Propanediol: 98%, Acros Chemical Company • 1,2-Butanediol: 99%, Aldrich Chemicals Company • 2,3-Butanediol: 98%, Aldrich Chemicals Company • 1,4-Butanediol: 99%, Aldrich Chemicals Company Chemicals used for carboxymethylation:
• Sodium Hydroxide: 50%, Fisher Chemicals Company • Sodium Carbonate: Reagent grade
Chemicals used for titration:
• Silver Nitrate: 1N solution, Fisher Chemicals Company
• Phenolphthalein: Powder, Baker and Adamson Chemicals Company
• Hydrochloric Acid: 0.09%, Fisher Chemicals Company
• Sodium Hydroxide: 0.2%, Fisher Chemicals Company
Chemical used for washing:
• Nonionic Surfactant: Kieralon MFB, BASF Chemicals Company
Chemicals used for bleaching:
• Sodium Hydroxide: 50%, Fisher Chemicals Company
• Ethylene Diamine Tetraacetic Acid (EDTA): Questal Special, BASF
• Wetting agent: Nonionic surfactant, Kieralon N-F, BASF Chemical Company • Stabilizer: Sodium silicate, Prestogen N-D, BASF Chemicals Company Chemicals used for durable press (DP) finishing:
• Modified Ethylene Urea Resin: Freerez 900 Reactant, Noveon Chemicals Company
• MgCl2 and AlCl3 catalyst: Freecat Accelerator, Noveon Chemicals Company
• Wetting Agent: Renex 36, Noveon Chemicals Company
Chemicals used for dyeing:
• Acid Dyestuff: CI Acid Red 114, Polar Red RS 125%, Ciba Chemical Company
• Basic Dyestuff: CI Basic Blue 3, Maxilon Blue 5G 200%, Ciba Chemical Company
• Acetic Acid: Glacial, 99.8%, Fisher Chemicals Company
3.2 Equipment for Preparation 3.2.1 Stirring hot plate
A Fisher Hot Plate was used to control the heating and stirring during synthesis of cationic crosslinker.
3.2.2 pH meter
A Fisher Scientific Co. model 600-pH meter was equipped with a standard combination pH electrode for measuring and adjusting pH before and after all synthesis reaction steps.
3.2.3 Padding machine and oven
Wet application of chemical materials was performed using a 35 cm laboratory pad machine manufactured by Werner Mathis AG. For drying and curing, samples were pinned on 18 X 30 cm metal pin frames and put in a forced air oven manufactured by Werner Mathis AG.
3.3.1 CIE whiteness index and dyeability
CIE Whiteness Index and CIE L*, C*, h* measurements of the fabrics were performed according to AATCC Standard Test Method 110 by using a Spectraflash SF600X, a double beam spectrophotometer, manufactured by DataColor, with 16mm area view, CIE standard illuminant D65 and 10o observer .
Titrations were carried out to find the carboxymethyl content of the fabrics by following the method offered by Hashem, Hauser and Smith in their previous study . Anionic cotton fabric was cut into small pieces; 100mL of 0.5% aqueous HCl solution prepared and fabric samples were steeped in it for 16 hours. The samples were then washed several times with cold deionized water until free from HCl and having a pH of 7. Silver nitrate drop test was performed to make sure there was no presence of chloride on the samples. The samples were dried at 105oC for 3 hours in laboratory type oven. Samples weighing approximately 0.25g were soaked in 25mL
of 0.05N aqueous NaOH solutions at room temperature for 4 hours. First, a blank solution was titrated with 0.05N aqueous HCl solution. Phenolphthalein pH indicator was used. The volume of HCl solution (mL) spent was recorded for the blank. Then, each of the solutions with different carboxymethylated samples was titrated in the same way as the blank. The carboxymethyl (CM) contents of samples were calculated as follows:
CM content (mmoles/100 grams) = 100 . (Vblank-Vsample)HCl . NHCl /0.25 (3.1)
where Vblank is the volume of HCl used for titration of blank solution, Vsample is the
volume of HCl used for titration of sample solution, and NHCl is the normality of HCl
Carboxymethyl content is a measure of anionic sites in the cellulose chain. Knowing the mmole CM content per 100 grams of cotton and as molecular weight of anhydro glucose unit is 162g/mole, we can easily calculate the average amount of anionic sites per anhydro glucose unit (AGU) as follows:
Average Number of anionic sites per AGU =
= CM content (mmole/100g) . 162(g/mole)/(1000mole/mmole*100g)
Average Number of AGUs per Anionic Site = 1/(CM content . 0.00162) (3.3)
where CM content is the carboxymethyl content in mmole/100g cotton.
3.3.3 Wrinkle recovery angle
WRA tests were done according to AATCC Test Method 66, option 2 . 12 specimens of 40 x 12mm are cut, six with their long dimension parallel to the warp direction of the fabric and six with their long dimension parallel to the filling direction. Warp specimens are cut from sample locations with different warp yarns and filling specimens are cut from sample locations with different filling yarns. We used a template for cutting the specimens and tweezers for handling them. Prior to testing samples are brought to moisture equilibrium in a standart atmosphere having a relative humidity of 65±2% at 21±1oC.
Each specimen is placed between the leaves of the metal holder with one end aligned under the 18mm marks using the tweezers. The free end of the specimen is lifted up and over to the 18mm mark taking care to loop back rather than flatten the specimen. The edge of the specimen is firmly hold in place with a thumbnail. The jaws of the plastic press is opened with the other hand. The holder with the specimen is inserted between the long and short jaws, releasing the thumbnail when bringing the end edge of the long jaw into contact with the specimen. The 18mm mark on the metal holder, the unfolded end of the specimen and the end edge of the plastic press are aligned before releasing the specimen. A fold should be formed 1.5mm from the end of the short metal leaf. The plastic press should be in firm contact with the folded specimen but should not be squeezed. The press-holder combination is inverted on a flat surface with the small platform up. 500g of weight is gently applied to the platform. After 5 minutes, the weight is removed and the press-holder combination is picked up by the plastic press and the exposed end of the specimen holder is inserted in the clip mount on the face of the recorder device. Jaws are opened and press is removed rapidly taking care to avoid rolling the exposed end of the specimen or pulling it out of the holder. The holder is aligned with the front edge of the clip mount shelf. The specimen fold should line up with the spot at the center of the recorder disc leaving the free hanging leg of the specimen aligned with the vertical guide line on the scale. To eliminate gravitational effects, the free hanging leg of the specimen is kept aligned with the recorder’s vertical guide line during the 5 minutes recovery period. Adjustments are made once every 15 seconds in the first minute and once every minute thereafter during the remaning recovery period. The final adjustment is made 15 seconds before the 5 minutes recovery period ends. The recovery angle is red from the scale and recorded. If the free end of a specimen twists, a vertical plane through its center is sighted and it is aligned with the vertical mark on the recorder scale.
Stiffness was determined using ASTM D 1388-96 . A Fabric Development Drape-Flex Stiffness Tester was used. This test method involves sliding a 2.5 cm by 15 cm specimen off the edge of a planar surface. The distance is recorded at which the fabric bends under its own weight to touch a surface extending at a 41.5o from the
edge. From this distance and the basis weight (average weight of the test fabrics) of the fabric, the bending rigidity is calculated.
3.3.5 Breaking strength, elongation and energy to peak load
Breaking strength tests were done with a Syntech tensile strength tester according to ASTM D5034 . Elongation and energy to peak load values were recorded as well.
The cotton fabric was tested for absorbency according to AATCC Test Method 79-1986 before and after bleaching . Prior to testing samples are brought to moisture equilibrium in a standart atmosphere having a relative humidity of 65±2% at 21±1oC. Fabric is mounted in the embroidery hoop so that the surface is free of wrinkles, but without distorting the structure of the material. The hoop is placed 10mm below the tip of the burette and one drop of distilled water at 21±3oC is allowed to fall on the fabric. Using the stopwatch, the time required, up to 60 seconds, for the surface of the liquid to lose its specular reflectance is measured. 5 reading are taken and their average is calculated.
3.3.7 Scanning electron microscope (SEM)
In order to investigate the effect of ionic crosslinking on breaking behavior of the fiber, we broke cotton yarn samples and had images of broken fibers by using SEM.
3.3.8 Nitrogen content
As the crosslinking agent comprised nitrogen, it is expected that the nitrogen content of ionic crosslinked fabric compared to that of untreated fabric would be higher. The nitrogen content of ionic crosslinked sample is a measure of the amount of crosslinks it has.
In order to determine the nitrogen content of our ionic crosslinked samples, a LECO TruSpec® CHN analyzer is used with the following settings; Air pressure: 40psi; He pressure: 35psi; O2 pressure: 38psi; Furnace Temperature: 950oC; After Burner
For calibration of this analyzer a standard EDTA (supplied by LECO) having 41.03±0.12% of carbon, 5.55±0.03% of hydrogen, and 9.57±0.04% of nitrogen is used.
Fabric samples are wrapped in capsules (supplied by Leco) of 8.0mm diameter and 20mm height. The samples are burned by using He and O2. After burning, the
gaseous product is analysed in order to determine the carbon, hydrogen and nitrogen content of the sample.
The ionic crosslinked samples were tested for smoothness according to AATCC Test Method 128-1999 . An M272 SDL Atlas AATCC Wrinkle Recovery Tester is used. This test method involves wrapping a 15 cm by 28 cm specimen around the tester, lowering the top flange of the tester and placing 3500 grams weight on the top flange for 20 minutes. After the weights are removed, the specimen is hung vertically in the long (warp) direction in standard conditioned atmosphere for 24 hours prior to evaluation by three trained observers.
3.4 Synthesis of Cationic Agents
8 different cationic agents are synthesized using different alcohols. These alcohols are reacted with CHTAC (N-(3-chloro-2-hydroxypropyl) trimethylammonium chloride) in 1:8 mole ratios. Additionally glycol is reacted with CHTAC in 1:4 mole ratio using the same procedure and the final product was called Glycerin 1:4. The general procedure for synthesis of cationic agent is as follows (see Figure 3.1):
• Weigh CHTAC and add 5% NaOH dropwise into CHTAC while stirring to adjust pH value between 10 to 11 at room temperature (Solution A).
• Weigh alcohol and add 5% NaOH dropwise into this alcohol while stirring at room temperature to adjust the same pH value with Solution A (Solution B). • Add Solution A dropwise into Solution B while stirring at room temperature.
Measure and record the pH of the mixture.
• Fix water bath temperature at 50oC and stir this mixture for 16 hours in constant temperature at water bath, cool down to room temperature, adjust pH with 5% acetic acid to between 6 to 8.
• To find solid content, weigh 3g of this product, dry in oven at 70oC for 24 hours and weigh it again.
Glycerin N+ CH3 CH3 CH3 Cl OH N+ CH3 CH3 CH3 O Na OH
3-chloro-2-hydroxypropyl trimethyl ammonium chloride Epoxypropyl trimethyl ammonium chloride
N+ CH3 CH3 CH3 O
+Cationic Glycerin Cl Cl Cl (EPTAC) (CHTAC) O H O H OH O O O N+ CH3 C H3 CH3 O H N+ CH3 CH3 OH N+ CH3 CH3 OH CH3 C H3 Cl Cl Cl
We offered an alternative procedure for cationic agent preparation. According to this procedure, CHTAC and glycerin are weighed and mixed before setting pH at room temperature. The resulting product was called Glycerin New.
We also tried reacting CHTAC with its hydrolyzed form to reach a cationic agent. The procedure we offered was as follows:
• Add 1:1.5 mole ratio 50% NaOH dropwise into CHTAC, stir at 80oC for 4 hours to hydrolyze CHTAC.
• Add equal mole of NaOH into CHTAC dropwise in ice bath while stirring. • Add this second solution dropwise into first one in ice bath, measure pH; if
pH value is not between 10 to 11, add NaOH to set pH to between 10 to 11. • Adjust water bath temperature to 80oC and stir for 2 hours, cool down to
room temperature, measure pH, adjust pH with acetic acid to between 6 to 8.
3.5 Applied Processes
3.5.1 DMDHEU crosslinking
For comparison of effect of conventional durable press finishing on cotton fabric with that of ionic crosslinking, we prepared samples with a common durable press finish (DMDHEU). 1L of pad bath composed of 250g/L modified ethylene urea resin, 62.5g/L catalyst, 1g/L wetting agent and 686.5mL deionized water. Softener was not used. Fabric samples were padded to 80-90% wet pick up. Samples were dried for 5 minutes and cured for 2 minutes at 105Co and 177Co, respectively.
We bleached the fabric by using 3g/L NaOH, 6g/L H2O2, 1g/L ethylene diamine
tetraacetic acid (EDTA), 1g/L surfactant and 1g/L stabilizer in a Jet dyeing machine with a liquor ratio (L.R.) of 1:8. All chemicals were added to bleaching liquor and reaction was started at 30oC by a temperature increase of 3°C/min. After the reaction temperature of 98oC was reached, bleaching was followed for 1 hour. Bleached fabric was rinsed for 10min. Bleaching procedure is shown in Figure 3.2.